free online editions of InTech
Books and Journals can be found at
Part 1 Synthesis and Characterization of Graphene 1
Chapter 1 Self-Standing Graphene Sheets Prepared with
Chemical Vapor Deposition and Chemical Etching 3
Genki Odahara, Tsuyoshi Ishikawa, Kazuya Fukase,
Shigeki Otani, Chuhei Oshima, Masahiko Suzuki,
Tsuneo Yasue and Takanori Koshikawa
Chapter 2 Nucleation and Vertical
Growth of Nano-Graphene Sheets 21
Hiroki Kondo, Masaru Hori and Mineo Hiramatsu
Chapter 3 Synthesis of Aqueous Dispersion
of Graphenes via Reduction of Graphite
Oxide in the Solution of Conductive Polymer 37
Sungkoo Lee, Kyeong K. Lee and Eunhee Lim
Chapter 4 Supercritical Fluid Processing
of Graphene and Graphene Oxide 45
Dinesh Rangappa, Ji-Hoon Jang and Itaru Honma
Chapter 5 Graphene Synthesis, Catalysis with Transition
Metals and Their Interactions by Laser Photolysis 59
Bonex W Mwakikunga and Kenneth T Hillie
Part 2 Properties and Applications of Graphene 79
Chapter 6 Complex WKB Approximations in
Graphene Electron-Hole Waveguides in Magnetic Field 81
Chapter 7 Atomic Layer Deposition of High-k Oxides on Graphene 99
Harry Alles, Jaan Aarik, Jekaterina Kozlova,
Ahti Niilisk, Raul Rammula and Väino Sammelselg
Chapter 8 Experimental Study of the
Intrinsic and Extrinsic Transport
Properties of Graphite and Multigraphene Samples 115
J. Barzola-Quiquia, A. Ballestar, S. Dusari and P. Esquinazi
Chapter 9 Electronic Transport
Properties of Few-Layer Graphene Materials 141
S. Russo, M. F. Craciun, T. Khodkov,
M. Koshino, M. Yamamoto and S. Tarucha
Chapter 10 Large Scale Graphene by
Chemical Vapor Deposition:
Synthesis, Characterization and Applications 161
Lewis Gomez De Arco, Yi Zhang and Chongwu Zhou
Graphene, discovered in 2004 by A. K. Geim and K. S. Novoselov, is an excellent
electronic material, and has been considered as a promising candidate for the post-
silicon age. It has enormous potential in the electronic device community, for
example, field-effect transistor, transparent electrode, etc. Despite intense interest
and remarkably rapid progress in the field of graphene-related research, there is still
a long way to go for the widespread implementation of graphene. It is primarily due
to the difficulty of reliably producing high quality samples, especially in a scalable
fashion, and of controllably tuning the bandgap of graphene. This book provides
some solutions to the above-mentioned problems, and is divided into two parts. The
first part discusses the synthesis and characterization of graphene, and the second
part deals with the properties and applications of graphene.
This book is a collection of contributions made by many outstanding experts in this
field, and their efforts and time should be greatly appreciated. Also, I sincerely
thank the efficient and careful editing by Ms. Iva Simcic.
Research on graphene is a fast developing field, with new concepts and applications
appearing at an incredible rate. It is impossible to embody all the information
related to this subject in a single collection, and hopefully it could be of any help to
people who are interested in this field.
Prof. Jian Ru Gong
National Center for Nanoscience and Technology, Beijing,
Synthesis and Characterization of Graphene
Sheets Prepared with Chemical
Vapor Deposition and Chemical Etching
Genki Odahara1 et al. *
1Department of Applied Physics, Waseda University, Tokyo,
Recently, much attention has turned to the structural and electronic properties of carbon-
based materials. At present, especially, graphene is the hottest topics in condensed-matter
physics and materials science. This is because graphene has not only unusual properties
regarding extreme mechanical strength, thermal conductivity and 2-diemensional films, but
also peculiar electronic characteristics such as Dirac-particles with a linear dispersion,
transport energy gap and simply absorption coefficient of lights (Geim & Novoselov, 2007;
Nair et al., 2008). These unique properties mean it could have a wide array of practical uses.
In addition to monolayer graphene, few-layer graphene has been extensively studied. For
example, bi-layer graphene creates a band gap when an external electric field is applied
(Castro et al., 2007; Zhang et al., 2009).
Graphene sheets have been produced mainly by exfoliating graphene flakes from bulk
graphite and depositing them on the SiO2/Si substrate. However, the size and crystalline
quality are not easily controlled. Some groups have grown epitaxially graphene sheets on
SiC(0001) (Hibino et al., 2010), however the graphene layers have been widely distributed in
For last 20 years, on the other hand, we have grown graphene (and/or h-BN), hetero-
epitaxial sheets on various solid surfaces by chemical vapor deposition (CVD) or surface
segregation techniques, and investigated their atomic, electronic and phonon structures
(Oshima & Nagashima, 1997).
Fig. 1 shows a schematic diagram of growing processes of graphene and h-BN films by CVD
or surface segregation techniques on solid surfaces reported so far. We demonstrated that
the thickness of graphene, and the width of graphene nano-ribbons were controlled
precisely by adjusting the annealing temperature, exposure time of deposition gases and
choosing the substrate (Nagashima et al., 1994; Tanaka et al., 2002).
* Tsuyoshi Ishikawa1, Kazuya Fukase1, Shigeki Otani2, Chuhei Oshima1, Masahiko Suzuki3,
Tsuneo Yasue3 and Takanori Koshikawa3.
1 Department of Applied Physics, Waseda University, Tokyo, Japan,
2 National Institute for Materials Science, Tsukuba-shi, Ibaraki, Japan,
3 Fundamental Electronics Research Institute, Academic Frontier Promotion Center,
Osaka Electro-Communication University, Osaka, Japan.
Graphene – Synthesis, Characterization, Properties and Applications4
Fig. 1. A schematic diagram of growing processes of graphene and h-BN films by CVD or
surface segregation techniques on solid surfaces.
Fig. 2 shows a intensity peak ratio of XPS C1s to Ta 4p as a function of hydrocarbon
exposure during the graphene growth on TaC(111) (Nagashima et al., 1994). For the first
monolayer formation, an exposure of a few hundred langmuir (1L = 1×10-6 Torr sec) was
required. In comparison with the first monolayer formation, an extremely large exposure of
~8×105 L was necessary for the second layer growth, and the growth rate of the third layer
was much slower than that of the second one. This indicates that surface reactivity for
hydrocarbon dissociation is reduced at each stage of the formation of graphene overlayer.
Fig. 2. An intensity peak ratio of XPS C1s to Ta 4p as a function of exposure during the
graphene growth on TaC(111).
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 5
Because of the large difference in the growth rate, the thickness of the overlayer could be
precisely controlled by adjusting the exposure.
Fig. 3 shows typical low energy electron diffraction (LEED) patterns of monolayer graphene
and monolayer h-BN films on single-crystal surfaces. Depending on the interlayer interactions
between graphene and the substrate, three different configurations were known.
1. On Pt (111), the crystallographic orientations of the growing graphene does not align
with those of the substrate lattices because of the weak interlayer interaction (Fujita et
al., 2005). Fig 3 (a) shows the presence of diffraction ring segments, which indicate
rotational disorder of graphene domains.
2. On TaC (111), ZrC (111), Ni (100), Ni (755) and Pd (111), the incommensurate epitaxial
sheets grew because of the strong interlayer interaction; there are many extra diffraction
spots in the LEED patterns owing to the multiple diffraction with two different
periodicity in Fig. 3 (b) and (c) (Aizawa et al., 1990; Nagashima et al., 1993a, 1993b).
3. The exception is a graphene (or h-BN)-covered Ni (111) surface; a 1 x 1 atomic structure
appeared in the LEED pattern in Fig. 3 (d) and (e), because of the small lattice misfits
and the strong interlayer interaction: The graphene (or h-BN) grew in a commensurate
way to the substrate lattice by expanding the C-C bonds by 1.2% (by contracting the B-
N bonds by 0.4%) (Gamo et al., 1997a, 1997b).
Fig. 3. Typical LEED patterns of graphene and h-BN films on single-crystal surfaces.
Epitaxial films grew in a commensurate way to the Ni(111), and in incommensurate ways to
the other surfaces.
Fig. 4 shows the atomic structure of the graphene-covered Ni(111) clarified with a LEED
intensity analysis (Gamo et al., 1997a). The LEED intensity analysis indicated that one C atoms
of graphene situate at all the on-top site of the topmost Ni atoms, and at all the three-fold FCC
hollow sites. Hence, the grain boundaries of graphene islands disappeared if the surface is
completely covered with either graphene or h-BN. In fact, uniform scanning tunneling
microscopy (STM) images were observed on the h-BN-covered Ni(111) (Kawasaki et al., 2002).
Fig. 4. The atomic structure of the graphene-covered Ni(111) clarified with a LEED intensity
Graphene – Synthesis, Characterization, Properties and Applications6
Recently, we have studied the growth mechanism of graphene layers on Ni(111) surface.
In this chapter, we report the in-situ observation of the graphene growth of mono-, bi- and
tri-layers using carbon segregation phenomena on Ni(111) by low energy electron
microscopy (LEEM), which is a powerful technique to investigate thin films in mesoscopic
We also fabricated the self-standing graphene sheets by chemically etching the substrate
(Odahara et al., 2009). The chemical process to remove the Ni substrate makes it possible to
prepare a self-standing graphene sheets, which are characterized by scanning electron
microscopy (SEM) or transmission electron microscopy (TEM).
2. In-situ observation of graphene growth on Ni(111)
Graphene growth of mono-, bi- and tri-layers on Ni(111) through surface segregation was
observed in situ by LEEM (Odahara et al., 2011). The carbon segregation was controlled by
adjusting substrate temperature from 1200 K to 1050 K. After the completion of the first
layer at 1125 K, the second layer grew at the interface between the first-layer and the
substrate at 1050 K. The third layer also started to grow at the same temperature, 1050 K. All
the layers exhibited a 1 x 1 atomic structure. The edges of the first-layer islands were straight
lines, reflecting the hexagonal atomic structure. On the other hand, the shapes of the second-
layer islands were dendritic. The edges of the third-layer islands were again straight lines
similar to those of the first-layer islands. The phenomena presumably originate from the
changes of interfacial-bond strength of the graphene to Ni substrate depending on the
graphene thickness. No nucleation site of graphene layers was directly observed. All the
layers expanded out of the field of view and covered the surface. The number of nucleation
sites is extremely small on Ni(111) surface. This finding might open the way to grow the
high quality, single-domain graphene crystals.
2.1 Macroscopic single-domain monolayer graphene sheet on Ni(111)
The carbon segregation on Ni(111) surface to grow graphene sheets has already been
investigated in detail by Auger electron spectroscopy (AES) and LEED observations
(Shelton et al., 1974).
Fig. 5 shows an overview of these results. The surface carbon content in a logarithmic scale
is schematically shown against the temperature. Depending on the temperature, three
different surfaces are observed: surfaces covered with multilayer graphene, single-layer
graphene and the bare Ni substrate without graphene. Above the first critical temperature
Tc1 = 1170 K, most carbon atoms disappear at the surface, penetrating into the Ni substrate.
Below Tc1, on the other hand, the solubility of carbon in Ni is reduced and the carbon atoms
segregate to the surface, forming either single- or multi-layer graphene depending on the
temperatures. Below the second critical temperature Tc2 = 1070 K, multilayer graphene is
thermodynamically stable, and single-layer graphene is stable between Tc1 and Tc2. The
LEED patterns of the three surfaces exhibit sharp diffraction spots representing 1 1 atomic
structures, indicating that the graphene layers are commensurate with Ni(111) substrate.
The high-brightness LEEM used in this work was recently developed by Koshikawa and
others; a negative electrode affinity (NEA) photocathode operating in an Extreme High
Vacuum (XHV, ~10-10 Pa) chamber achieved high brightness of 107A cm-2 sr-1 (Jin et al., 2008;
Suzuki et al., 2010; Yamamoto et al., 2008).
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 7
Fig. 5. Surface carbon content versus substrate temperature of a graphene-Ni(111) system
(see Shelton et al., 1974). Depending on the temperature, there exist three different surfaces;
multilayer coverage, monolayer coverage and bare Ni.
Fig. 6 shows snapshots from the LEEM time series after the temperature was decreased from
1200 K to 1125 K. Images (a)-(d) are 6μm field-of-view, and image (e) is 100μm field-of-view.
Letters (a) to (d) in each image represents the time-lapse order during the observing period
of about 3 minutes from (a) to (d). Two white domains of monolayer graphene appeared
and expanded gradually as shown in images (a)-(b) and met each other in images (c)-(d). We
can see clearly the straight lines at the island edges, which cross with each other by either
60° or 120° reflecting the hexagonal structure of graphene. Correctly describing, the angles
are not exactly 60° and 120°, because the graphene sheets are not perfectly flat and curved
along the substrate surface. Graphene sheet grew continuously across the steps in carpet-
like fashion, and slightly curved at the steps.
Growing directions of graphene islands were always perpendicular to the linear edges
independent of the surface structures; the Ni(111) substrate surface possesses steps with a
few nm amplitudes produced by polishing as seen clearly in image (e). The graphene sheets
grew continuously beyond the steps.
In images (c)-(d), they were united to form one graphene sheet without any grain
boundaries. Finally, the observed area was entirely covered with monolayer graphene. We
observed carefully whole the substrate surface of several centimeters in scale, but no grain
boundaries were found by LEEM.
All the μLEED patterns observed in the graphene-covered surface showed a 1 x 1 structure
as shown in image (f). The graphene sheets were flat and epitaxial on the terraces. The
orientation was slightly altered at the steps because of the slight curving of the graphene
sheet. It is strong contrast to the fact that the μLEED patterns of the bare substrate exhibited
sharp diffraction spots without streaks. Namely, single-domain epitaxial sheet grew
continuously across the steps. The slight streak in the μLEED pattern in image (f) reflects the
curving at the steps.
Graphene – Synthesis, Characterization, Properties and Applications8
Fig. 6. Typical snapshots of LEEM images obtained as the temperature was decreased from
1200 K to 1125 K (images (a) to (d)). The observed area was 6μm field-of-view. Letter in each
image indicates the time-lapse order. Two graphene domains were united to form one
graphene sheet. Image (e) is a typical LEEM image of 100μm field-of-view. The surface was
entirely covered with monolayer graphene. LEEM images were obtained at the primary
electron energy of 3.5 eV. Image (f) is a typical μLEED pattern observed in the graphene-
covered surface. The orientation of the graphene was slightly altered because the sheet is
In this several tenth times observation, no nucleus generation of the islands was directly
observed inside the LEEM sight at the maximum field of view, 100μm diameter. Graphene
islands always appeared out of the LEEM sight. It indicated that carbon diffusion rate was
high enough to find the energetically minimum positions as compared with generation of
other nucleus. That is, the number of nucleation sites is extremely small on Ni(111) surface.
The small number of nucleation sites is the most important factors of growing macroscopic
single-domain graphene crystals. When the graphene domains met each other, defects or
corrugations arise in the graphene crystals. Compared with other metals as graphene
growth substrates reported so far, Ni has the large solubility of carbon, about 0.5 at % at
1000K. Due to the large solubility of Ni, carbon atoms always segregate or penetrate into the
Ni bulk at 1125K. Few graphene islands, which exceed certain critical size, could continue to
grow by adopting the segregated carbon atoms. This might be the crucial reason why the
single-domain large graphene sheet grow on Ni(111) surface. On Ni(111) surface, as the
results, graphene sheets grew larger in carpet-like fashion independent of the morphology
of substrate surface from few nucleation sites. The domains were unified without
boundaries and wrinkles in the growth of the first layer on Ni(111) surface.
2.2 Bi- and tri-layer graphene growth on Ni(111)
Fig. 7 shows typical LEEM images at the different stages of the graphene growth, a typical
μLEED pattern obtained from the single-layer graphene-covered surface, and the electron
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 9
reflectivity-energy curves obtained from each area: (a)-(b) the first-layer growth at 1125K,
(d)-(f) the second-layer growth at 1050K and (g)-(h) the third-layer growth at 1050K. In Fig.2
(a)-(b), the growth rate of the first layer was faster than those of the second and third layers.
The growth rate of the first layer was about 10μm/s.
Fig. 7. Typical LEEM images of the graphene growth at different stages: (a)-(b) the first layer
growth observed at 1125K, (d)-(f) the second layer at 1050K and (g)-(h) the third layer at
1050K. Image (c) is a typical μLEED pattern of a 1 x 1 atomic structure obtained from the
single-layer graphene-covered surface. Image (i) is the electron reflectivity-energy curves
obtained from each area.
Fig. 7 (c) is a typical μLEED pattern of a 1 x 1 atomic structure obtained from the single-
layer graphene-covered surface. Similar μLEED patterns of a 1 x 1 atomic structure were
obtained from the bi- and tri-layer graphene-covered surface, showing the epitaxial sheets.
After the growth of the first layer was completed, we decreased the temperature from 1125
K to 1050 K to grow the second and third layers. Differing from the smooth edge of the first-
Graphene – Synthesis, Characterization, Properties and Applications10
layer islands, the shape of the second-layer shown in Fig.7 (d)-(f) was dendritic; namely, the
shape was determined kinetically owing to the anisotropic carbon diffusion depending on
the morphology of substrate surface. The second layer grew preferentially along the
morphology of the Ni substrate because of the different interfacial space owing to the first
layer curving: The interfacial interaction of the first layer is stronger than the Van-der-Waals
bonds in bulk graphite crystals, and the second layers have to cut into the interface between
the first layer and the substrate to grow. This might be the reason of the slow-growth rate of
the dendritic islands. The growth rate was about 10 times slower than that of the first layer;
the growth rate of the second layer is about 1 μm/s. The second-layer grew also in carpet-
like fashion independent of the morphology of substrate surface. In addition, like the first-
layer growth, no nucleus generation of the second-layer islands was found even in the
maximum 100μm field-of-view. The second-layer domains always appeared out of the
LEEM sight. The second-layer domains were also unified without boundaries and wrinkles.
Bi-layer graphene domains grew at least 100μm scale at 1050 K.
The interesting phenomenon was observed concerning the growth of the third layer, when
we kept the temperature at 1050 K. The third layer also started to grow at a few places as
shown in Fig.7 (g)-(h). The shape of the islands reflects the hexagonal atomic structure.
Namely, straight lines of the island edges crossed with each other by 120°, similar to the
first-layer growth. However, the growth rate is not so fast compared with that of the first-
layer growth. The growth rate of the third layer is about 0.1μm/s. The carbon diffusion rate
at the interface should be slower than that on the bare Ni surface, but carbon diffusion was
isotropic independent of the substrate structures. Fig. 7 (i) shows the electron reflectivity-
energy curves obtained from each area. The number of graphene layers can be counted
directly as the number of dips in the reflectivity. The electronic energy bands of graphene
sheet are quantized with sheet thickness, and possesses valleys in the energy range of 3-9 eV
of the reflection curves. The valley originates from increases in the electron transmission
owing to the occupied bands of graphene sheet. The valley numbers and their energy
positions are changed systematically depending on the thickness such as monolayer, bi-
layer, tri-layer, etc (Hibino et al., 2010).
In previous papers, we reported the weakening of the interfacial interaction with the metal
substrate by the second-layer covering the first-layer through CVD technique. For example,
double-layer graphene on TaC(111) and hetero-epitaxial system (monolayer
graphene/monolayer h-BN) on Ni(111) (Kawasaki et al., 2002; Nagashima et al., 1994;
Oshima et al., 2000).
Fig. 8 shows typical LEED patterns of two types of surfaces: (a) a monolayer h-BN on
Ni(111), and (b), (c) the double atomic layers of graphene and a monolayer h-BN on Ni(111).
The pattern (c) was obtained by a CCD camera with an exposure time five times longer than
that used for the patterns (a) and (b). In the pattern (a), we observed sharp diffraction spots
exhibiting a 1 × 1 atomic structure. Intensive LEED spots in the pattern (b) exhibiting a 1 × 1
atomic structure, together with new weak features, which are clearly seen in the pattern (c).
We observed faint rings and additional spots at the positions that are rotated by 30° from
those of the Ni(111) substrate. The ring radius and positions of the additional spots agreed
with the reciprocal lattice of the graphene sheets, while the graphene overlayer did not have
a perfect epitaxial relation to the pristine monolayer h-BN/Ni(111); namely, the graphene
overlayer had domains with different azimuthal angles. Fig. 9 shows typical tunneling
dI/dV spectra of (a) h-BN/Ni(111), (b) graphene/h-BN/Ni(111) and (c) highly oriented
pyrolytic graphite (HOPG). The metallic characters appeared for (a) h-BN/Ni(111) in the
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 11
spectrum reflecting the strong interfacial interaction. However, the additional graphene
coverage changed the spectra to the non-linear curve at zero bias, exhibiting a feature of
either semiconductor or insulator.
Fig. 8. Typical LEED patterns of (a) h-BN/Ni(111) and (b), (c) graphene/h-BN /Ni(111). The
pattern (c) was obtained for a longer exposure, while the pattern of (B) was measured for
Fig. 9. Typical tunneling dI/dV spectra of (a) h-BN/Ni(111), (b) graphene/h-BN/Ni(111)
and (c) HOPG. The metallic characters appeared for (a) h-BN/Ni(111).
Additional two experimental indications were observed in electronic and vibrational
structures. With respect to the interfacial bonding, the first-layer graphene interacts with
TaC(111) substrate, with modified π branches of electronic structure and reduced work
function. Owing to the coverage of the additional second layer, the modified π branches
returned to the bulk-like π branch, which indicated that interfacial interaction became weak
similar to that in bulk graphite (Nagashima et al., 1994).
Another one was vibrational frequency change of phonons; the interfacial interaction
reduces transverse optical (TO) frequencies of the first-layer by 20 % from the bulk ones on
Graphene – Synthesis, Characterization, Properties and Applications12
Ni(111), while the additional graphene coverage returned the TO phonon frequencies to the
bulk ones. All the three data described above indicated that the additional layer on the first
layer weakens the interfacial interaction (Oshima et al., 2000).
The phenomenon of the third-layer growth observed by LEEM is consistent with the above
data. The interfacial space of the bi- layer and substrate might not be as narrow as that of the
single-layer and substrate, estimated 0.21 nm by means of LEED intensity analysis as shown
in Fig. 4 (Gamo et al., 1997a). In the wide space, the segregated carbon atoms can find the
energetically minimum positions similar to the case of the first-layer growth, and as a result,
the equilibrium shape appeared at the third-layer growth.
We also observed interesting phenomena of moving wrinkles in the second layer growth at
1050 K, which were shown in Fig.10 . Image (a) of Fig.10 is a raw LEEM image, image (b) is
the mofified image of (a) using a frame substraction method; the substraction-intensity
difference between two sequent frames are protted in two dimensions in order to emphasize
the moving wrinkles. We can see clearly the wave-like motions of wrinkles by eliminating
the non-moving static substrate structures, which are black thick lines in image (a). Image (c)
is the same image as (b) with adding the superimposed lines, which are guides for the eye
indicating the moving wrinkles. The superimposed arrow indicates the direction of the
second-layer growth and the smoothing direction of the wrinkles. The wrinkles moved the
same direction as that of the second-layer growth. This wrinkles motions appeared just after
the formation of the second layer, and the wrinkles disappeared gradually, which means
that the origion of the wrinkles was stress relaese generated by the formation of the second
layer, such as the mismach of lattice constant, stacking and change in the interfacial
interaction between graphene and Ni(111). This phenomena are related with the motions of
whole the large garphene sheet, which means that carpet-like growth occurs in the wide
Fig. 10. A typical smoothing in the second layer growth at 1050 K. Image (a) is a raw
LEEM image, (b) is the same image as (a) using frame difference method to emphasize the
moving wrinkles, and remove the static substrate structures (black thick lines in image
(a)). Image (c) is the same image as (b) added the superimposed lines. The superimposed
arrow indicates the direction of the second-layer growth and the smoothing direction of
Fig. 11 shows the mean-square amplitudes of thermal atomic vibrations of graphite(0001)
surface as a function of electron energy, which were obtained from Debye-Waller factors
measured on the basis of the temperature dependence of LEED intensity (Wu et al., 1985).
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 13
With decreasing the incident electron energy, the atomic vibration amplitudes became
larger due to the high sensitivity of the graphite surface. This indicates that the thermal
vibrational amplitudes of surface atoms are larger than that of the bulk crystal interior.
However, the surface phonon dispersion curves of graphite measured with HREELS are
almost the same in bulk. Hence, only the origin of the large vibrational ampulitude
indicated by LEED is attributed to the phonons at long wavelength as comapred with
atomic distance. These phonons cannot be detected by HREELS because their wave
vectors are too small around Γ point, and their vibrational energires are too low . That is
to say, whole the surface sheet moves largely, which is in good agreement with the direct
observations of wrinkle motion. We concluded that the second-layer seems to grow at the
interface, vibrating and stretching the wrinkles. In addition, if there are many grain
boundaries in the second-layer, the wrinkle stretch easily stops at the boundaries. Since
the wrinkle motion continued during the growth of the second layer, the single-domain
second layer might grow in large scale.
Fig. 11. The effective mean-square atomic vibration amplitudes of graphite(0001) surface as
a function of electron energy (see Wu et al., 1985).
3. Self-standing graphene sheets
Additional chemically etching the Ni substrate made it possible to separate macroscopic
self-standing graphene sheets with a few tenth mm in size (Odahara et al., 2009). Self-
standing sheets could be the ideal sample support of organic materials for TEM
observations. Low-energy electron microscope together with holder made of graphene
sheets seems to be promising for observation of organic- and/or bio-materials.
Fig. 12 shows a typical TEM images (a) of the carbon aggregates at 100 kV. Because we
detected only the spots of graphene sheets in diffraction patterns, we concluded that the
observed materials are composed of multi-folding graphene sheets. In Fig. 12 (a), the
Graphene – Synthesis, Characterization, Properties and Applications14
squares of the Au mesh are 10 μm × 10 μm in area, and the carbon aggregate in Fig. 12 (a)
is a few tenth mm in scale. The magnified image of the thinnest area of the aggregate is
shown in Fig. 12 (b). The uniform films covered one of the square holes of the mesh. Fig.
12 (c) is the diffraction patterns of the uniform area of Fig. 12 (b). Only sharp diffraction
spots of graphene were observed, and moreover, no Ni signals were detected in X-rays
Fig. 12. (a) A TEM image of a carbon aggregate on the Au mesh with squares 10 μm × 10 μm
in area, (b) A magnified TEM image of the thinnest area of the carbon aggregate, and (c) its
electron diffraction pattern.
Fig. 13 shows (a) the TEM image of a slightly thicker area and (b) its diffraction pattern. All
the spots are split in doublets in Fig. 13 (b). The observed area is covered with double-layer
graphene sheets, of which the crystal orientations differs by 9 ゜ each others.
We saw several diffraction patterns indicating different folding structures. Hence, the
double layer seems to be formed by chance during the removing the Ni substrate.
In the TEM image of the double-layer sheets, we observed CNT-like structures appeared as
shown in Fig. 11 (a). The origin of the structure is not clear now.
Fig. 14 shows the 532 nm Raman spectrum of the monolayer self-standing sheets. The two
intense features are the G peak at ～1580cm-1 and the 2D peak at ～2700 cm-1. The single and
sharp 2D peak in image indicates that the self-standing sheet has a thickness of only one
atomic layer (Ferrari et al., 2006). In addition, small defect-origin D peak was detected at
～1350 cm-1. This proves that the high-quality graphene grows on Ni(111), which could be
transferred to other substrates.
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 15
Fig. 13. A TEM image of the other area in the carbon aggregate (a) and its diffraction pattern
(b). One can see clearly doublets of diffraction spots in (b), and new cabon-nano-tube like
structures in (a). The hole was covered with double-layer graphene.
Fig. 14. Typical Raman spectrum of the monolayer self-standing graphene sheets. Small
defect-origin D peak was detected at ～1350 cm-1.
Graphene – Synthesis, Characterization, Properties and Applications16
Lastly, we have one comment that the graphene is a promising material supporting bio-
molecules for TEM observations. In Fig. 15 and Fig. 16, we showed the transmission electron
diffraction patterns of a single-layer graphene measured with different electron energies of
5, 1 and 0.5 kV. With decreasing the electron energy, the ratios of diffraction spot intensity to
the background intensity, and the (00) spot intensity to the (01) intensity became small,
because the sensitivity of light elements change.
Fig. 15 are the SEM image of single graphene sheet at 5 kV and its Low Energy-
Transmission Electron Diffraction (LETED) pattern at 5kV. Compared with TEM image, we
can clearly observe the graphene surface by SEM.
Fig. 15. The SEM image of single graphene sheet at 5 kV and its LETED pattern (upper
Fig. 16 shows the LETED pattern of graphene at (a) 1 kV and (b) 500 V. When we decreased
the electron energy down from 1 kV to 500 V, the intensity of the (10) spot increased
compared with that of the (00) spot because of large elastic scattering cross section of
electrons by graphene. Adsorbed molecules on graphene sheet also increase the intensity of
the diffuse scattering.
Fig. 17 is (a) the SEM image of folding double graphene sheet and its LETED pattern at (b) 4
kV and (c) 2kV. When we decreased the electron energy down from 4kV to 2kV, the
additional satellite spots (white circles in image (b)) due to the double diffraction appeared
in the patterns because of the large elastic scattering cross section.
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 17
Fig. 16. The LETED pattern of single-layer graphene at (a) 1 kV and (b) 500 V.
Fig. 17. The SEM image of folding double graphene sheet (a) and its LETED pattern at (b) 4
kV and (c) 2kV.
The Ni(111) surface is the excellent substrate for growth of single-layer-graphene sheet with
macroscopic dimensions. Graphene sheets with a 1 x 1 atomic structure grew up epitaxially
by CVD or surface segregation techniques.
We in-situ observed the graphene growth of mono-, bi- and tri-layer step by step using
carbon segregation phenomena on Ni(111) by LEEM. The summaries are as follows;
1. One can grow the uniform monolayer graphene on Ni(111) by adjusting the
temperature. No domain boundaries and wrinkles were detected by LEEM.
2. The second- and the third-layer graphene grew at the interface under the first and the
second layers. Bi-layer graphene domains grew at least 100μm scale. The third-layer
started to grow before the completion of second-layer at 1050K in this experiment. More
precise control of temperature seems to be required to complete the second-layer before
starting the third-layer growth.
Graphene – Synthesis, Characterization, Properties and Applications18
3. Shape of the islands differed depending on the thickness; the first- and third-
layer islands exhibit hexagonal edges, while the second-layer islands possess dendritic
4. The different shapes of the first, second and third-layer islands presumably originate
from the interfacial-bond strength depending on the graphene thickness.
5. The number of nucleation sites of graphene growth is extremely small on Ni(111)
surface, which is an important factor for growth of large single-domain graphene
6. Chemical etching the Ni substrate made it possible to separate macroscopic self-
standing graphene sheets.
M. S, T. Y and T. K are grateful for the partial support from Grants-in-Aid for Scientific
Research (A) (No. 19201022).
Aizawa, T.; Souda, R.; Otani, S.; Ishizawa, Y. & Oshima, C. (1990). Anomalous bond of
monolayer graphite on transition-metal carbide surfaces. Phys. Rev. Lett. Vol.64 pp.
Castro, E. V.; Novoselov, K. S.; Morozov, S.V.; Peres, N. M. R.; Lopes dos Santos, J. M. B.;
Nilsson, J.; Guinea, F.; Geim, A. K. & Castro Neto, A. H. (2007). Biased Bilayer
Graphene: Semiconductor with a Gap Tunable by the Electric Field Effect. Phys.
Rev. Lett. Vol.99, pp. 216802-1 - 216802-4.
Ferrari, A. C.; Meyer, J. C.; Scardaci, V.; Casiraghi, C.; Lazzeri, M.; Mauri, F.; Piscanec, S.;
Jiang, D.; Novoselov, K. S.; Roth, S. & Geim, A. K. (2006). Raman Spectrum of
Graphene and Graphene Layers. Phys. Rev. Lett. Vol.97 pp. 187401-1 - 187401-4.
Fujita, T.; Kobayashi, W. & Oshima, C. (2005). Novel structures of carbon layers on a Pt(111)
surface. Surf Interface Anal Vol.37 pp. 120-123.
Gamo, Y.; Nagashima, A.; Wakabayashi, M.; Terai, M. & Oshima, C. (1997a). Atomic
structure of monolayer graphite formed on Ni(111). Surf. Sci. Vol.374 pp. 61-64.
Gamo, Y.; Terai, M.; Nagashima, A. & Oshima, C. (1997b). Atomic Structural Analysis of a
Monolayer Epitaxial Film of Hexagonal Boron Nitride/Ni(111) studied by LEED
Intensity Analysis. Sci. Rep. RITU A44 pp. 211-214.
Geim, A. K. & Novoselov, K. S. (2007). The rise of graphene. Nature Mater Vol.6, pp. 183-
Hibino, H.; Kageshima, H. & Nagase, M. (2010). Epitaxial few-layer graphene: towards
single crystal growth. J. Phys. D: Appl. Phys. Vol.43 pp. 374005 1-14.
Jin, X.; Yamamoto, N.; Nakagawa, Y.; Mano, A.; Kato, T.; Tanioku, M.; Ujihara, T.; Takeda,
Y.; Okumi, S.; Yamamoto, M.; Nakanishi, T.; Saka, T.; Horinaka, H.; Kato, T.; Yasue,
T. & Koshikawa, T. (2008). Super-High Brightness and High-Spin-Polarization
Photocathode. Appl. Phys. Express Vol.1 pp. 045002-1-045002-3.
Kawasaki, T.; Ichimura, T.; Kishimoto, H.; Akber, A. A.; Ogawa, T. & Oshima, C. (2002).
Double atomic layers of graphene/monolayer h-BN on Ni(111) studied by scanning
Self-Standing Graphene Sheets Prepared with Chemical Vapor Deposition and Chemical Etching 19
tunneling microscopy and scanning tunneling spectroscopy. Surf. Rev. Lett. Vol.9
Nagashima, A.; Itoh, H.; Ichinokawa, T. & Oshima, C. (1994). Change in the electronic
states of graphite overlayers depending on thickness. Phys. Rev. B, Vol.50 pp. 4756-
Nagashima, A.; Nuka, K.; Itoh, H.; Ichinokawa, T. & Oshima, C. (1993). Electronic states of
monolayer graphite formed on TiC(111) surface. Surf. Sci. Vol.291 pp. 93-98.
Nagashima, A.; Nuka, K.; Satoh, K.; Itoh, H.; Ichinokawa, T. & Oshima, C. (1993). Electronic
structure of monolayer graphite on some transition metal carbide surfaces. Surf. Sci.
Vol.287/288 pp. 609-613.
Nair, R. R.; Blake, P.; Grigorenko, A. N.; Novoselov, K. S.; Booth, T. J.; Stauber, T.; Peres, N.
M. R. & Geim, A. K. (2008). Fine Structure Constant Defines Visual Transparency of
Graphene. Science Vol.320, pp. 1308.
Odahara, G.; Ishikawa, T.; Otani, S. & Oshima, C. (2009). Self-Standing Graphene Sheets
Prepared with Chemical Vapor Deposition and Chemical Etching. e-J. Surf. Sci.
Nanotech. Vol.7 pp. 837-840.
Odahara, G.; Otani, S.; Oshima, C.; Suzuki, M.; Yasue, T. & Koshikawa, T. (2011).
In-situ Observation of Graphene Growth on Ni(111). Surf. Sci. Vol. 605 pp. 1095-
Oshima, C. & Nagashima, A. (1997). Ultra-thin epitaxial films of graphite and hexagonal
boron nitride on solid surfaces. J. Phys.: Condens. Matter Vol.9 pp. 1-20.
Oshima, C.; Itoh, A.; Rokuta, E.; Tanaka, T.; Yamashita, K. & Sakurai, T. (2000). A hetero-
epitaxial-double-atomic-layer system of monolayer graphene/monolayer h-BN on
Ni(111). Solid State Commun. Viol.116 pp. 37-40.
Shelton, J. C.; Patil, H. R. & Blakely, J. M. (1974). Equilibrium segregation of carbon to a
nickel (111) surface: A surface phase transition. Surf. Sci. Vol.43 pp. 493-520.
Suzuki, M.; Hashimoto, M.; Yasue, T.; Koshikawa, T.; Nakagawa, Y.; Konomi, T.; Mano, A.;
Yamamoto, N.; Kuwahara, M.; Yamamoto, M.; Okumi, S.; Nakanishi, T.; Jin, X.;
Ujihara, T.; Takeda, Y.; Kohashi, T.; Ohshima, T.; Saka, T.; Kato, T. & Horinaka, H.
(2010). Real Time Magnetic Imaging by Spin-Polarized Low Energy Electron
Microscopy with Highly Spin-Polarized and High Brightness Electron Gun. Appl.
Phys. Express Vol.3 pp. 026601-1-026601-3.
Tanaka, T.; Tajima, A.; Moriizumi, R.; Hosoda, M.; Ohno, R.; Rokuta, E.; Oshima, C. &
Otani, S. (2005). Carbon nano-ribbons and their edge phonons. Solid State Commun.
Vol.123 pp. 33-36.
Wu, N. J.; Kumykov, V. & Ignatiev, A. (1985). Vibrational properties of the graphite (0001)
surface. Surf. Sci. Vol.163 pp. 51-58.
Yamamoto, N.; Nakanishi, T.; Mano, A.; Nakagawa, Y.; Okumi, S.; Yamamoto, M.; Konomi,
T.; Jin, X.; Ujihara, T.; Takeda, Y.; Ohshima, T.; Saka, T.; Kato, T.; Horinaka, H.;
Yasue, T.; Koshikawa, T. & Kuwahara, M. (2008). High brightness and high
polarization electron source using transmission photocathode with GaAs-GaAsP
superlattice layers. J. Appl. Phys, Vol.103 pp. 064905-1 - 064905-7.
Graphene – Synthesis, Characterization, Properties and Applications20
Zhang, Y.; Tang, T-T.; Girit, C.; Hao, Z.; Martin, M. C.; Zettl, A.; Crommie, M. F.; Ron Shen,
Y. & Wang, F. (2009). Direct observation of a widely tunable bandgap in bilayer
graphene. Nature Vol.459 pp. 820-823.
Nucleation and Vertical
Growth of Nano-Graphene Sheets
Hiroki Kondo, Masaru Hori and Mineo Hiramatsu
Nagoya University, Meijo University
Carbon nanomaterials, such as carbon nanotubes (CNTs), graphene sheets and so forth,
have attracted much attention for not only scientific interest but also various application
expectations. For example, various applications of CNTs, such as field emitter, transistor
channel, and so forth, have been proposed, because of their unique nanostructures, excellent
electrical and physical properties.[1-3] Graphene sheets are also promising candidates as
channel materials of electronic devices, since both electron and hole in them have extremely
high carrier mobilities (10,000–15,000 cm2/Vs). Carbon nanowalls (CNWs) are one of such
self-aligned carbon nanomaterials. They consist of graphene sheets standing vertically on
substrates as shown in Fig.1. Significant recent attention has been focused on the
functionalities of CNWs for future devices because of their unique morphologies and
excellent electrical properties. For example, since they have large surface-to-volume ratios
and very high aspect ratios, they are expected as catalyst supporting materials in fuel cells,
field emitters, and various kinds of templates [5-7]. In addition, the recent reports of
extremely high carrier mobilities in graphene sheets suggest that the CNWs would also
possess excellent electrical properties. Therefore, the CNWs are also expected to be applied
to high-carrier-mobility channels and low-resistivity electrodes in next-generation electronic
For the practical applications of CNWs, it is indispensable to control their morphologies
and electrical properties. And, to establish such the controlled synthesis techniques of
CNWs, it is essential to clarify their growth mechanisms. For the synthesis of the CNWs,
the plasma-enhanced chemical vapor deposition (PECVD) systems are used in most cases
and no catalyst is necessary for its growth [5-11]. However, their growth mechanisms
have not been sufficiently clarified yet. Tachibana et al. reported interesting results of
crystallographic analysis on carbon nanowalls, in which preferential orientations of
graphene sheets change with the growth time. On the other hand, more fundamental
mechanisms of CNW growth, such as nucleation of nanographene, and relationships
between plasma chemistry and CNW growth, are poorly understood. It is due to the
complicated growth processes in the plasma. In this study, we investigated roles of
radicals and ions in the growth processes of CNWs by distinctive inventions on the
originally-developed Multi-beam PECVD systems and precise measurements of active
species during the growth processes.
Graphene – Synthesis, Characterization, Properties and Applications22
Fig. 1. (a) Top-view SEM image and (b) schematic illustrations of typical CNWs.
2. Initial growth processes of carbon nanowalls
When the growth of the CNWs is performed by the PECVD for different growth times, it
can be found that there are the series of events leading up to the formation of CNWs. A 10
nm thick interface layer composed of carbon nanoislands was firstly formed on the Si
substrate for a short time, and then CNWs growth began from the nuclei on the interface
layer . In order to realize the industrial applications of CNWs with unique
characteristics, it is very important to understand the growth mechanism of the initial layer
and CNWs to achieve control of the characteristics and morphologies that are appropriate to
each application [5-7]. Moreover, the nucleation of CNWs in the very early phase must be
very important for control of the characteristics and morphology. The following questions to
be solved are; why are the morphologies changed from an interface layer (nanoislands) to
CNWs under homogeneous conditions, and why do vertical CNWs grow from flat interface
layers. To answer these questions, the surface conditions suitable for CNW growth were
investigated using a multi-beam chemical vapor deposition (CVD) system and the
correlation between the nanoislands and CNW growth was investigated.
A rapid and simple preparation process is desirable for industrial applications. On the other
hand, it is also very important to separate each growth phase, formation of the nanoislands,
nucleation, and CNW growth, to elucidate these mechanisms. However, it is difficult to
separate these growth phases because the formation of nanoislands and nucleation proceed
within a very short duration with plasma-enhanced CVD (PECVD). Moreover, the
conditions for nanoisland formation and nucleation are almost the same as that of the
subsequent CNW growth. Therefore, we have focused on the early phases, and established
two different conditions for nanoisland formation and CNW growth starting with the first
incidence of graphene (nucleation). In this study, a pretreatment was introduced for the
formation of nanoislands, and the effects of the pretreatment process on CNW growth were
investigated. CNWs are grown on an amorphous carbon (a-C) interface layer including the
nanoislands. The optimum surface conditions for nucleation of CNWs are discussed in the
2.1 Multi-beam chemical vapor deposition system and two-step growth technique
As mentioned above, the nucleation of nanographene occurs at the very early phase of
CNWs growth generally. Therefore, it is very difficult to detect it when we use the
conventional PECVD system. In addition, it is also hard to clarify roles of each radicals or
ions at the PECVD processes, since fluxes and energies of each active species are not
Nucleation and Vertical Growth of Nano-Graphene Sheets 23
independently-controllable in the conventional PECVD system. Therefore, in this study, we
employed the multi-beam CVD system having independently-regulated two radial sources
and one ion source. Using this system, the effects of each active species on nucleation and
vertical growth of nanographene during the formation of the CNWs can be systematically
2.1.1 Multi-beam chemical vapor deposition system
Figure 2 shows the schematic diagram of multi-beam CVD system. This system consists of 3
beams of carbon-containing radicals, hydrogen radicals, and ions. Two radical sources
(fluorocarbon and H radicals) were mounted obliquely at the upper right and left sides of
the reactive chamber, and C2F6 and H2 gases were introduced into the radical sources
separately. The identical radical sources consist of radio frequency (rf: 13.56 MHz)
inductively coupled plasma (ICP) with spiral coil and grounded metal meshes in the head to
retard irradiating electrons and ions. Orifices were installed in the head of fluorocarbon
radical source and H radical source, respectively, in order to control the flux of radicals.
Radicals generated in these sources irradiated a substrate with the angle of 30° from the
horizontal line. On the other hand, the ion source was mounted on the top of the reactive
chamber. The ion source consists of 13.56 MHz rf ICP. The plasma potential in the ICP was
set to 0‒250 V by applying DC voltage. A metal mesh connecting to the ground was
installed inside the ion source. Generated Ar+ ions were accelerated between the ICP and the
mesh, and irradiated vertically a substrate. The ion current is measured using Faraday cup.
CF3 radical H radical
Fig. 2. Schematic diagram of multi-beam CVD system.
Graphene – Synthesis, Characterization, Properties and Applications24
The process gases and irradiated active species are pumped out by a turbo molecular pump,
and the total pressure is controlled by a gate valve. The base pressure was approximately
1.0×10-4 Pa. A substrate is introduced onto the stage in the center of the chamber, where
irradiations of all species were focused on. When CNWs are synthesized, the substrate is
heated by a carbon heater beneath the lower electrode and the substrate temperature is
measured by an optical pyrometer and ellipsometric analysis. In-situ spectroscopic
ellipsometry is available in this system. Xe lamp and the detector were installed on the
windows in the side wall of the chamber in opposed position with the angle of 15° from the
horizontal line. This spectroscopic ellipsometer would obtain some information of the
growing materials in real time. Measured ellipsometric data were calculated and fit by using
a personal computer.
200 300 400
Ar ion source power (W)
Fig. 3. Counts of CF3
+ ions ionized from CF3 radicals as a function of Ar+ ion source power.
Independent controllability of this system was confirmed by quadrupole mass spectrometry
(QMS).[15-17] Figure 3 shows the signal (counts) of CF3
+ ion ionized from CF3 radicals
obtained by QMS as a function of rf-ICP power of Ar+ ion source. The intensity did not
significantly change. Any other relations such as fluorocarbon radical vs H radicals showed
the similar behaviours. From the result, the irradiations can be independently controlled.
2.1.2 Two-step growth technique
CNW growth was carried out using the multi-beam CVD system. Two different deposition
sequences for CNW growth were performed and are indicated in Table 1. The first is a
single-step growth with constant irradiation conditions of the Si substrates (no
pretreatment), and the second is a two-step growth on Si substrate. In the two-step growth,
the first step is a 15 min pretreatment and the second step is CNW growth for 35 min,
wherein the gas flow rate, ICP power, and Ar+ ion acceleration voltage and flux are varied.
The Ar+ flux in the second step was varied from 1.8 to 5.4 μA/cm2 by changing the ICP
power, and the ion energy was varied from 160 to 250 eV by changing the DC voltage.
Combinations of irradiation with fluorocarbon radicals, H radicals, and Ar+ ions were
Nucleation and Vertical Growth of Nano-Graphene Sheets 25
varied in the pretreatment step. In contrast, the conditions of the second step (subsequent
CNW growth) were not changed to analyze the effects of the pretreatment.
Table 1. Growth conditions
C2F6, H2, and Ar gases were used to generate fluorocarbon radicals, H radicals, and Ar+ ions,
respectively. For the pretreatment step, the flow rates of the C2F6, H2, and Ar gases were 5, 6,
and 10 sccm, respectively, and the ICP power for the generation of fluorocarbon radicals, H
radicals, and Ar+ ions were 200, 200, and 300 W, respectively. The reflection powers were
less than 10% of forward powers. In the fluorocarbon radical source, CF3 radicals were
predominantly generated. The gases with reactive species were pumped out using a turbo
molecular pump through a gate valve. During the pretreatment, the total gas pressure
ranged between 0.4 and 2.0 Pa, which was dependent on the combination of irradiation
species (i.e. no operation of the gate valve between experiments with different variations of
irradiation species). Si substrates were introduced to the center of the stage and the surface
temperature was kept at 580°C during the 15 min pretreatment process.
After pretreatment, CNW growth was conducted using the multi-beam CVD system under
identical conditions. Ar+ ion, fluorocarbon radical, and H radical sources were also used and
generated from Ar, C2F6 and H2 gases, respectively. The powers of each source were 300,
200, and 200 W, respectively, and the flow rates of Ar, C2F6, and H2 were 5, 10, and 6 sccm,
respectively. The surface temperature was maintained at 580°C during the 35 min growth
Following the CNW growth process, samples were observed using a scanning electron
microscope (SEM). For some samples, scanning tunneling microscopy (STM) was also
conducted. Additionally, in situ spectroscopic ellipsometry was performed throughout the
pretreatment and the CNW growth processes.
Graphene – Synthesis, Characterization, Properties and Applications26
2.2 Initial growth processes of CNWs
Morphological changes of growth surfaces in the initial phase, and their dependence on the
growth conditions are discussed in this chapter. Pre-deposition of carbon layers including
nanoisland structures and their morphologies are closely-correlated with following growth
of CNWs. Especially, effect of Ar+ ion irradiation on nanoislands formation at the first step
2.2.1 Morphological changes of growth surfaces
Figures 4(a) and 4(b) show tilted-view scanning electron microscopy (SEM) images of
samples prepared by single-step growth for (a) 15 min and (b) 50 min. In Fig. 5.1(a),
several nanoislands approximately 10 nm in diameter and 5 nm in height are evident on the
substrate. X-ray photoelectron spectroscopy (XPS) results have shown that these
nanoislands are mainly composed of carbon atoms and a small amount of fluorine. In
contrast, CNWs were formed after 50 min growth, as shown in Fig. 4(b). Thus, it was
confirmed that CNWs were synthesized by the multi-beam CVD system and also by
conventional plasma-enhanced CVD.
Fig. 4. Tilted-view SEM images of samples formed by single-step growth for (a) 15 and (b) 50
min. Insets show top-view SEM images for each sample.
2.2.2 Effects of nanoislands formation on CNWs growth
Two-step growth was conducted to investigate the nucleation and growth of CNWs
separately. Figures 5(a) and (b) show tilted-view STM images of samples after pretreatment
with and without Ar+ irradiation, respectively. In the case of Ar+ irradiation, nanoislands
were observed on the substrate, as shown in Fig. 5(a). Their size and chemical composition
were similar to those of the nanoislands shown in Fig. 4(a). In contrast, no nanoislands were
obtained without Ar+ irradiation (Fig. 5(b)). It should be noted that CNWs were never
obtained during the pretreatment step, even if performed with or without Ar+ irradiation for
50 min, which indicates that the irradiation conditions of the ions and radicals required for
CNW growth are different from those for nanoisland formation. Figures 5(c) and (d) show
tilted-view SEM micrographs of samples grown by the two-step process, where the first step
pretreatments were performed with and without Ar+ irradiation, as shown in Figs. 5 (a) and
(b), respectively, and where in the second step, the Ar+ flux was increased to 3.8 µA/cm2 at
an energy of 200 eV under the same densities of H and CF3 radicals as those for single-step
growth. It is significant that CNWs are only grown (Fig. 5(c)) when Ar+ irradiation is used in
Nucleation and Vertical Growth of Nano-Graphene Sheets 27
the pretreatment step, while only a continuous film was obtained for growth after
pretreatment without Ar+ irradiation (Fig. 5(d)). These results indicate that energetic Ar+
irradiation during the pretreatment (initial growth process) is necessary for CNW growth,
and the nucleation of CNWs is incubated in the nanoislands by high density Ar+ irradiation.
Therefore, nucleation and CNW growth could be clearly distinguished using the two-step
Fig. 5. Tilted-view STM images of samples after pretreatment for 15 min (a) with and (b)
without Ar+ irradiation. Tilted-view SEM images of samples formed by two-step growth, in
which pretreatments were performed (c) with and (d) without Ar+ irradiation.
2.3 Effects of H radicals on CNW growth
The effects of radicals were investigated in a multi-beam CVD system. The H2 gas flow rate
was changed from 0 to 10 sccm in the second step (CNW growth), and C2F6 and Ar gas flow
rates were kept constant at 10 and 5 sccm, respectively. Therefore, several different
composition ratios of H/C or H/CF3 would be obtained under these conditions. The
chamber was evacuated through a gate valve using a turbo molecular pump, and the total
gas pressure was controlled at 2.5 Pa by the valve when the H2 gas flow rate was 5 sccm.
The valve position was not changed at various H2 gas flow rates in order to maintain the
fluxes of Ar+ ions and CFx radicals. Therefore, the total pressures ranged from 2.2 to 2.8 Pa at
H2 flow rates from 0 to 10 sccm. The rf ICP powers applied to H radical source, fluorocarbon
source, and Ar+ ion source were 200, 200, and 300 W, respectively. The irradiation period for
each sample was 35 min.
2.3.1 Morphological dependence of CNWs on H radicals
Figures 6(a)–(e) show tilted-view SEM images of CNWs synthesized for 35 min at different
H2 gas flow rates of (a) 0, (b) 3, (c) 5, (d) 7, and (e) 10 sccm. When the H2 gas flow rate was 0
Graphene – Synthesis, Characterization, Properties and Applications28
sccm, the ICP power for H radical generation was not applied. No CNWs were formed
without irradiation by H radicals, but a very thin layer was apparent on the Si substrate, as
shown in Fig. 6(a). Figure 6(b) shows that for a H2 gas flow rate of 3 sccm, nanoparticles
rather than CNWs were deposited. In contrast, when the H2 gas flow rate was increased up
to 5 sccm, CNWs were densely grown during the initial phase. In these samples, the
distance between adjacent CNWs was approximately 10 to 20 nm, and the thickness of the
CNW sheet was less than 5 nm. With further increase of the H2 gas flow rate to more than 10
sccm, no CNWs were grown, as shown in Fig. 6(e).
50 nm(d) (e)
Fig. 6. Tilted-view SEM images of samples synthesized for 35 min at H2 gas flow rates of (a)
0, (b) 3, (c) 5, (d) 7, and (e) 10 sccm.
Figure 7 shows the variation of CNW height measured from the cross-sectional SEM
images as a function of the H2 gas flow rate. The height of CNWs increased with the H2
gas flow rate. The highest CNWs (approximately 48 nm) were obtained at a H2 gas flow
rate of 5 sccm. Further increase of the H2 gas flow rate resulted in a decrease of the CNW
height. It should be noted that at H2 gas flow rates greater than 10 sccm, CNWs were
etched, which was confirmed by the following experiment: CNWs were synthesized in
advance at a H2 gas flow rate of 7 sccm (as shown in Figs. 6(d)), and the substrate with
CNWs was again introduced into the multi-beam system. H radicals (H2: 10 sccm or more)
and other species (C2F6 at 10 sccm, Ar at 5 sccm and accelerated at 200 eV) were irradiated
onto the CNW sample. As a result, the height of the CNWs was reduced with increase in
the process time. The very thin layer evident in Fig 6(e) was probably deposited when all
irradiation was ceased and the conditions of each species would change for just a
Nucleation and Vertical Growth of Nano-Graphene Sheets 29
0 5 10 15
H2 gas flow rate (sccm)
Fig. 7. Height of CNWs as a function of the H2 gas flow rate.
Vacuum ultraviolet absorption spectroscopy (VUVAS) was applied to measure the absolute
density of H radicals during simultaneous irradiation with CFX radicals, H radicals, and Ar+
ions.[18-20] The procedure to estimate the H radical density was described in detail in ref. 17-
19. Figure 8 shows that the H radical density increased almost linearly with the H2 gas flow
rate, and the highest density of 4.3×1011 cm-3 was obtained at a H2 gas flow rate of 7 sccm.
0 2 4 6 8 10
H2 gas flow rate (sccm)
Fig. 8. Absolute density of H radicals as a function of the H2 gas flow rate measured using
Graphene – Synthesis, Characterization, Properties and Applications30
However, the H radical density appeared to decrease with further increase of the H2 gas
flow rate above 7 sccm, which was rather due to the device limitation; it was difficult to
efficiently maintain ICP at high flow rates and high pressures. The results shown in Figs. 6–8
suggest that the H radical density has a strong influence on the nucleation and morphology
of the resulting CNWs, and there would be an optimum ratio of H radical density to
fluorocarbon flux or other species. Moreover, it is noted that CNWs were not formed at a H2
gas flow rate of 10 sccm, although the H radical density was almost the same as that at 5
sccm. It is presumed that in the case of high flow rate of H2 gas, the dissociation rate from H2
molecules to H atoms was low and/or by-products containing H, such as HF and CHx, were
generated. Under such conditions, H2 molecules would disturb the transport of other
important species and chemical reactions. In addition, by-products related to H would
influence the amount of CFx radicals present, which has an important role for CNW growth
when using a fluorocarbon/hydrogen system. Therefore, further investigation regarding the
role of H2 molecules is required.
2.3.2 Compositional dependence of CNWs on H radicals
Figure 9 shows atomic composition ratios measured by XPS for CNWs grown at different
H2 flow rates during a simultaneous irradiation process. The composition ratios of F/C
and Si/C were estimated from the intensities of the C 1s, F 1s, and Si 2p peaks using
ionization cross-section value of each peak. It should be noted that difference in electron
inelastic mean free path of each photoelectron and that in surface roughness are not
considered at this estimation. Therefore, although absolute values of estimated
composition ratios are not precise, qualitative tendencies can be discussed based on them.
0 2 4 6 8 10
H2 gas flow rate (sccm)
Fig. 9. Atomic composition ratios of CNWs grown at different H2 flow rates. The flow rates
of C2F6 and Ar were 10 and 5 sccm, respectively.
Nucleation and Vertical Growth of Nano-Graphene Sheets 31
At H2 gas flow rates of 5–7 sccm, where CNWs were definitely formed, a large amount of C
was contained mainly in the deposits, while F and Si were rarely detected, which indicates
that the Si substrate was fully covered with carbon nanostructures, despite irradiation with
fluorocarbon radicals. On the other hand, even when CNWs were not obtained (H2 gas flow
rates of 0 and 10 sccm), F and C were detected, which suggests that a fluorocarbon
monolayer is present on the Si substrates. There is also a correlation between the heights of
the CNWs shown in Fig.7 and the F contents in the deposits; CNWs with increased height
contain lower F content. It is well known that H atoms scavenge F atoms, which results in
the formation of by-products such as HF. CNWs were rarely formed at a low H2 flow rate of
3 sccm or less, because F atoms on the top of the growing CNWs were not sufficiently
scavenged. In contrast, CNWs were not formed at a high density of H atoms, because excess
H atoms would remove both F and C atoms from the growth surface. Even when CNWs
were grown at H2 gas flow rates of 5–7 sccm, not all F atoms were scavenged, which
suggests that other parameters, such as the acceleration voltage, flux of Ar+ ions, and the
surface temperature require optimization.
2.4 Effects of ions on CNW growth
The effects of ions on CNW growth were investigated in a multi-beam CVD system. A first
subject is what type of combination of radicals and ions is effective on the initial growth of
CNWs. Various combinations of radicals and ions were employed to the first-step at the
two-step growth. Secondly, dependence of CNW growth on energy and flux of ions are
discussed. Energy and flux of ions during the second step were varied, and changes in
surface morphologies of deposits are studied.
2.4.1 Synergetic effects of radicals and ions on CNW growth
The combinations of irradiation species used in the pretreatment step were varied. The
pretreatment step consisted of irradiation with Ar+ ions and/or fluorocarbon radicals
and/or H radicals. In all samples, in situ ellipsometry revealed that CNWs were not
obtained only by the pretreatment step. The CNW growth process was then carried out for
35 min after pretreatment without exposure to the atmosphere between the pretreatment
and CNW growth steps.
Figure 10 shows tilted-view SEM images of the samples after the pretreatment and the CNW
growth processes. In Fig. 10, pretreatments were composed of irradiation with (a) energetic
Ar+ ions at 200 eV (Ar+), (b) CF3 radicals (CF3), (c) H radicals (H), (d) Ar+ + CF3, (e) Ar+ + H,
(f) CF3 + H, and (g) Ar+ + CF3 + H. The conditions for the CNW growth process (second
step) were constant for all samples. As shown in Figs. 10(b), (c), and (f), no CNWs were
observed, but a thin film was obtained after the CNW growth process with pretreatments
consisting of CF3, H, and CF3 + H. In contrast, CNWs were successfully formed on the Si
substrates after CNW growth with pretreatments of Ar+, Ar+ + CF3, Ar+ + H, and Ar+ + CF3
+ H, as shown in Figs. 10(a), (d), (e), and (g), respectively. It is noted that CNWs were
formed only when irradiation with Ar+ ions was included in the pretreatment. The CNW
heights were different for each sample; however, it is not meaningful to estimate the growth
rate, due to the different starting time of CNW growth. In contrast, the morphologies were
almost the same when CNWs were obtained, as shown in Figs 10(a), (d), (e), and (g). From
SEM observations, it is considered that irradiation with Ar+ is crucial for subsequent CNW
growth; irradiation with Ar+ is one of the key factors for the formation of Si substrate
conditions ideal for CNW growth.
Graphene – Synthesis, Characterization, Properties and Applications32
Fig. 10. Tilted-view SEM images of samples after two-step growth on Si substrates.
The pretreatment step consisted of irradiation with (a) energetic Ar+ ions at 200 eV (Ar+)
(b) CF3 radicals (CF3), (c) H radicals (H), (d) Ar+ + CF3, (e) Ar+ + H, (f) CF3 + H, and
(g) Ar+ + CF3 + H. The conditions for the second step (CNW growth) were constant for
2.4.2 Dependence of CNW growth on energy and flux of ions
Figure 11 shows a chart of Ar+ ion irradiation and the effect on CNW growth in terms of
fluxes ranging from 1.8 to 5.4 µA/cm2 and energies ranging from 160 to 250 eV. The
variation in morphology is classified in three areas in the chart; CNW formation, continuous
film formation, and no deposition, as indicated in Fig. 10 by dark gray, light gray and white
backgrounds, respectively. In this figure, heights (h) of grown films are also indicated. At an
Nucleation and Vertical Growth of Nano-Graphene Sheets 33
Ar+ ion energy of 200 eV, the heights of grown films increase with increasing the Ar+ ion
flux. This means absorption enhancement of CF3 radicals by ion irradiation. It is deduced
that the ion flux determines the amount of dangling bonds produced on the growth surface.
The rate of dangling bond production should be lower than the rate of nucleation site
production in order to induce vertical growth of nanographene sheets and result in CNW
growth. On the other hand, at an Ar+ ion flux of 3.8 A/cm2, the heights of grown films
decrease with increasing the Ar+ ion energy. This indicates etching effects of the grown films
by the ion irradiation. Therefore, the ion energy is also a critical factor for CNW growth,
because its strength determines the production of dangling bonds, nucleation, and etching.
Therefore, Ar+ irradiation conditions with limited fluxes (3.3–3.8 µA/cm2) and energies
(200–250 eV) along with CF3 and H densities in the order of 1011 cm-3 must be critical factors
for CNW growth.
1.8 3.3 3.8 4.5 5.4
Ar+ ion flux (µA/cm2)
h=12 nm h=18 nm h=25 nm h=25 nm
h=25 nm h=25 nm
(c) (d) (e) (f)
No deposition Film
Fig. 11. Chart of Ar+ ion irradiation for CNW growth for fluxes ranging from 1.8 to 5.4
µA/cm2 and ion energies ranging from 160 to 250 eV. The height (h) of each sample is
indicated in each SEM image.
The roles of fluorocarbon radicals and hydrogen radicals are discussed. At the top of the
growing CNW, the edge would be terminated by CF3. A H radical migrates to the edge and
the terminated F atom at the top is removed by abstraction with a H radical. The HF
molecule generated is exhausted to the gas phase. At the same time, dangling bonds are
generated on C atoms and CF3 radicals from the fluorocarbon radical source or migrating on
the CNWs are absorbed at the dangling bonds. As a result, a new C-C bond is produced.
Repetition of these processes results in CNW growth. It is considered that graphitization
would be affected by high energy ion irradiation as well as thermal assist.
Graphene – Synthesis, Characterization, Properties and Applications34
In this experiment, the CF3 density (nCF3) during CNW growth was evaluated to be
approximately 4.6–9.2×1011 cm-3 by QMS. The H radical density (nH) was evaluated to be
approximately 4.0×1011 cm-3 by VUVAS. These experimental results show nH/nCF3 ranges
from 0.4–0.9 when CNWs are grown. Furthermore, three H radicals are needed to abstract
all fluorine from a CF3 molecule. However, since the sticking coefficient of CF3 radicals to
the surface is relatively low, fluorine atoms of absorbed CF3 radicals would be sufficiently
abstracted by H radicals under the present growth conditions with high temperatures.
These fundamental results and discussion are relevant to conventional PECVD methods that
employ C2F6/H2 or CH4/H2 gases, where mainly CFx
+ or CHx
+ ions are irradiated. Details of
atomic-level surface reactions at the CNW growth are still under investigation, and further
investigations with more accurate experiments are required to solve them. However, it is
expected that preferable structures and morphologies of CNWs could be formed through a
fundamental understanding of the synergetic effects of the radicals and ions on the chemical
reactions at the edges and surfaces of CNWs.
Mechanisms of nucleation and vertical growth of nanographenes at the initial growth of
CNWs were described in this study. Especially, effects of radicals and ions irradiated to the
growth surfaces on the initial growth of CNWs were intensively discussed based on plasma
chemistry analyzed by advanced diagnostic techniques.
CNWs were synthesized by irradiation with energetic Ar+, fluorocarbon and H radicals in a
multi-beam CVD system. Fluxes and energies of radicals and ions can be independently
controlled. During the initial growth of CNWs, the irradiation conditions required for the
nucleation of nanographenes are found to be different from those required for their vertical
growth. Ar+ irradiation is required to form both a-C nanoislands for subsequent nucleation
of nanographene on the nanoislands. On Si substrates, SEM observations revealed that
irradiation with Ar+ ions is effective for the initial nucleation process for CNW growth. In
addition, irradiation with CF3 and H radicals is also effective to promote nucleation. From
these results, nanoisland formation and CNW growth were successfully distinguished, and
the effects of nanoisland formation on nucleation process of nanographene were
CNWs were successfully synthesized by simultaneous irradiation of CFX radicals, H
radicals, and Ar+ ions, and it was confirmed that Ar+ ions were necessary to form CNWs.
The growth mechanism and critical factors for CNW growth were quantitatively revealed as
follows: low energy Ar+ cannot induce the nucleation of CNWs, and very high energy Ar+
enhances the etching of surface carbon atoms. Only under Ar+ ion irradiation with
appropriate energies (200–250 eV) and fluxes (3.3–3.8 µA/cm2), and with CF3 and H
densities in the order of 1011 cm-3, the CNWs are formed. No deposit is found on the
substrate without H radical irradiation. With respect to the H2 gas flow rate, CNWs were
grown at 5–7 sccm, where the H radical density was approximately 4.0×1011 cm-3. The CF3
radical density was evaluated by QMS to be approximately 5–9×1011 cm-3. XPS results
indicated that H radicals also have an important role in the abstraction of F atoms from
absorbed CF3 on CNWs.
These results indicate that a multi-beam CVD system is a powerful tool for fundamental
experiments to solve complicated growth mechanisms of carbon nanostructures employing
PECVD. Advanced diagnostics of plasma chemistry are also indispensable to make
Nucleation and Vertical Growth of Nano-Graphene Sheets 35
quantitative discussions about surface reactions during the growth. On the other hand,
appropriate plasma conditions necessary for nucleation and vertical growth of
nanographenes at the PECVD processes of CNW are determined. It is expected that these
results will be very useful for the controlled synthesis of CNWs with preferred
morphologies and characteristics.
This work was partly supported by Ministry of Education, Culture, Sports, Science and
Technology, Regional Innovation Cluster Program (Global Type) “Tokai Region
Nanotechnology Manufacturing Cluster”, Japan.
 Iijima, S. (1991). Nature, Vol. 354, pp. 56-58.
 A. G. Rinzler, J. H. Hafner, P. Nikolaev, L. Lou, S. G. Kim, D. Tomanek, P. Nordlander,
D. T. Cobert and R. E. Smalley (1995). Science, Vol. 269, pp. 1550-1553.
 Seidel, R. V. ; A. P. Graham ; Kretz, J. ; Rajasekharan, B. ; Duesberg, G. S. ; Liebau, M.;
Unger, E. ; Kreupl, F. & Hoenlein W. (2005). (2009). Nano Lett., 2005, 5 (1), pp 147–
 Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang, Y.; Dubonos, S. V.;
Grigorieva, I. V. & Firsov, A. A. (2004). Science, vol. 306, pp. 666-669.
 Wu, Y. H. ; Qiao, P. W. ; Chong, T. C. & Shen, Z. X. (2002). Adv. Mater., vol. 14, pp. 64-67.
 Hiramatsu, M.; Shiji, K. ; Amano, H. & Hori, M. (2004). Appl. Phys. Lett., vol. 84, pp. 4708-
 Takeuchi, W.; Ura, M.; Hiramatsu, M.; Tokuda, Y.; Kano, H. & Hori, M. (2008). Appl.
Phys. Lett., vol. 92, pp. 2131031-21310313.
 Wang, J. J.; Zhu, M. Y.; Outlaw, R. A.; Zhao, X.; Manos, D. M.; Holloway, B. C. &
Mammana, V. P. (2004). Appl. Phys. Lett., vol. 85, pp. 1265-1267.
 Sato, G.; Morio, T.; Kato, T. & Hatakeyama, R. (2006). Jpn. J. Appl. Phys., vol. 45, pp. 5210-
 Chuanga, A. T. H.; Boskovicb, B. O. & Robertson, J. (2006). Diamond Relat. Mater., vol. 15,
 Kobayashi, K.; Tanimura, M.; Nakai, H.; Yoshimura, A.; Yoshimura, H.; Kojima, K. &
Tachibana, M. (2007). J. Appl. Phys., vol. 101, pp. 094306-1-094306-4.
 Yoshimura, H.; Yamada, S.; Yoshimura, A.; Hirosawa, I.; Kojimaa, K. & Tachibana, M.
(2009). Chem. Phys. Lett., vol. 482, pp. 125-128.
 Kondo, S.; Kawai, S.; Hori, M.; Yamakawa, K.; Den, S.; Kano, H. & Hiramatsu, M. (2009).
J. Appl. Phys., vol. 106, pp. 094302-1-094302-6.
 Kondo, S.; Kondo, H.; Hiramatsu, M.; Sekine, M. & Hori, M. (2010). Appl. Phys. Expr.,
vol. 3, pp. 045102-1-045102-3
 Sugai, H. & Toyota, H. (1992). J. Vac. Sci. Technol. A, vol. 10, pp. 1193-1200.
 Hikosaka, Y., Nakamura, M. & Sugai, H. (1994). Jpn. J. Appl. Phys., vol. 33, pp. 2157-2163.
 Hori, M. & Goto, T. (2002). Appl. Surf. Sci., vol. 192, pp. 135-160.
 Takashima, S.; Arai, S.; Hori, M.; Goto, T.; Kono, A.; Ito, M. & Yoneda, K. (2001).
J.Vac.Sci.Technol., vol.A19, pp.599-602.
Graphene – Synthesis, Characterization, Properties and Applications36
 Flaherty, D. W.; Kasper, M. A.; Baio, J. E.; Graves, D. B.; Winters, H. F.; Winstead, C. &
McKoy, V. (2006). J. Phys. D: vol. 39, pp.4393-4399.
 Takeuchi, W.; Sasaki, H.; Kato, S.; Takashima, S.; Hiramatsu, M. & Hori, M. (2009). J.
Appl. Phys., vol. 105, pp. 113305 -1- 113305 -6.
Synthesis of Aqueous
Dispersion of Graphenes via
Reduction of Graphite Oxide in the
Solution of Conductive Polymer
Sungkoo Lee, Kyeong K. Lee and Eunhee Lim
Korea Institute of Industrial Technology
Graphene is a quasi–two-dimensional material. Two-dimensional conductor graphene
has recently attracted attention due to in-plane mechanical, thermal, and electronic
properties as well as its applications in future optoelectronic devices. These excellent
properties may be relevant at the nanoscale if graphite can be exfoliated into thin
nanoplatelets, and even down to the single graphene sheet level. Recently, the size of
graphene films produced is limited to small sizes because the films are produced mostly
by exfoliating graphite, which is not a scalable technique. Graphene sheets were produced
by chemical reduction of exfoliated graphite oxides [1-5]. Hydrophilic graphite oxide was
prepared by oxidation of pristine graphite [6,7] and it has functional groups such as
epoxide, diol, ether, ketone, and hydroxyl groups. These functional groups in graphite
oxide impart water solubility to the individual sheets. Solution processable graphite oxide
has been used to fabricate paper like films with excellent mechanical properties, as well as
electrically conductive polymeric composites . But because of these functional groups,
graphite oxide is electrically insulating. High conductivity graphene nanosheets were
prepared via chemical reduction process of graphite oxide to graphite. But in the process
of reduction, reduced graphite flakes agglomerate and eventually precipitate. This
precipitated graphite flakes could not be re-dispersed by sonication in water containing
surfactants. To avoid agglomeration of grapheme, other host polymers such as poly(4-
styrenesulfonic acid) must be used, which hamper the electron-transfer property of the
The solution processing compatibility of graphenes make the material attractive for large
area applications. But chemically reduced GO films showed low conductivities as high as 0.5
S/cm. However such level of conductivity is not sufficient for transparent electrode
applications. So, we explore the direct preparation method of graphene solution by the
reduction of graphite oxide in the solution ionic conductive polymer. As a result, we
obtained a stable aqueous dispersion of graphene. The obtained graphene, coated with
conductive polymer, can be re-dispersed in water. The structural and electrical properties of
graphene were also examined with FT-IR, SEM, XPS, and 4-point probe conductivity
Graphene – Synthesis, Characterization, Properties and Applications38
2.1 Materials and methods
Graphite oxide was synthesized from natural graphite, obtained from Sigma-Aldrich
Company. Hydrazine hydrate was used for the reduction of graphite oxide. Deionized
water was used as solvent. Poly(4-styrenesulfonic acid) (PSS) and Nafion were used as
surfactants. These materials were obtained from Sigma-Aldrich Company.
PEDOT:PSS(Baytron P), was purchased as an aqueous dispersion from H.C.Starck,
Germany. The actual solid content in Baytron P is 1.5-2% according to the manufacturer. All
of the reagents were used as received without further treatment.
Fourier transform infrared (FT-IR) spectra were recorded in the range 400–4000 cm−1 with a
4 cm−1 resolution from KBr pellets on a Perkin-Elmer Spectrum. UV/Vis spectra of aqueous
graphene dispersion were collected using a Shimadzu UV-2550 UV/Vis spectrophotometer.
The chemical state and composition of the graphene thin films were examined by a Perkin
Elmer XPS (model PHI 5500) apparatus at a base pressure in the vacuum chamber lower
than 107 Pa. The mixture of PEDOT/PSS and polymer-coated graphene was prepared by
the solution of polymer-coated graphene adding into PEDOT/PPS solution and stirred for
1hr. The mixture was filtered with 0.45 μm Teflon filter before being used for spin coating.
The spin-coated film was dried at 120 ℃. Before spin coating, substrates were cleaned using
TCE, water, and ethanol. The film thickness was determined using Alpha-step. The sheet
resistance of films was measured by four-point probe method at room temperature.
2.2 Preparation of water-soluble graphene oxide (GO)
Graphene oxide was prepared using modified Hummers method from graphite . The
graphite was chemically oxidized by treatment with NaNO3, KMnO4, H2SO4, and H2O2, and
washed with mixed aqueous solution of 3wt% H2SO4 and 0.5wt% H2O2.
Impurities were removed by centrifugation. The final resultant water solution was passed
through a weak basic ion-exchange resin to remove the remaining HCl acid. Then water was
removed through a drying process. Finally, the brown powder was obtained.
2.3 Chemical reduction of graphite oxide
GO (100 mg) was dispersed in 100 ml of water. This dispersion was sonicated until it
became clear with no visible particulate matter. Hydrazine hydrate was added and the
solution was heated in an oil bath at 100 ℃ for 24 h. Reduced GO gradually precipitated out
as a black solid. This product was isolated by filtration and washing copiously with water.
The obtained reduced graphite oxide powder was dried on the vacuum oven at 150 ℃ for
24 h. This material could not be re-suspended even after prolonged ultrasonic treatment in
2.4 Nafion-coated graphite sheets via reduction of graphite oxide
GO (100 mg) was dispersed in 100 ml of water and the resulting suspension was sonicated
for 1 h. After adding Nafion to the aforesaid suspension and stirring for 4 h, hydrazine
hydrate was added to the above mixture. The mixture was continuously stirred at 100 ℃ for
24 h. As the reduction proceeds, color of polymer-coated graphite oxide change from brown
to black. The polymer-coated graphene was isolated via filtration with PVDF membrane
(0.45 μm pore size) and washed with water. Nafion-coated graphene can be re-dispersed in
water upon sonication, forming black suspensions.
Synthesis of Aqueous Dispersion of Graphenes via
Reduction of Graphite Oxide in the Solution of Conductive Polymer 39
2.5 PSS-coated graphite sheets via reduction of graphite oxide
GO (100 mg) was dispersed in 100 ml of water and the resulting suspension was sonicated
for 1 h. After adding poly(4-styrenesulfonic acid) to the aforesaid suspension and stirring for
4 h, hydrazine hydrate was added to the above mixture. The mixture was continuously
stirred at 100 ℃ for 24 h. As the reduction proceeds, color of polymer-coated graphite oxide
change from brown to black. The polymer-coated graphene was isolated via filtration with
PVDF membrane (0.45 μm pore size) and washed with water. PSS-coated graphene can be
re-dispersed in water upon sonication, forming black suspensions.
3. Results and discussion
The graphite oxide is electrically insulating. The conductivity of graphene can be obtained
by removal of the oxidized moieties in the graphite oxide by chemical reduction. But in the
process of reduction, reduced graphite flakes agglomerate and eventually precipitate. We
prepared the stable aqueous dispersions of graphite nanoplatelets by chemical reduction in
the aqueous polymer, Nafion or PSS. Figure 1 shows pictures of the water dispersion of
reduced graphite and PSS- and Nafion-coated graphene. Reduced graphite was not
dispersed in water but PSS-coated graphene (RGO-PSS) and Nafion-coated graphene (RGO-
Nafion) were dispersed readily in water. During reduction, Nafion (or PSS) interact with
platelets to compete with hydrophobic interaction between the graphite platelets. But once
Nafion (or PSS) is attached to the graphite platelet surface, agglomeration of the graphite
platelet is stopped .
Fig. 1. Water dispersions of reduced graphite oxide (a), reduced graphite oxide with PSS (b)
and Nafion (c)
Figure 2 shows the FT-IR spectra of GO before reduction, and after reduction without and
with PSS or Nafion. In figure 2a, a FT-IR spectrum of GO shows a broad absorption band at
3390 cm-1, which is related to the OH groups, and absorption bands at 1629 cm-1 and
1720 cm-1, which are typical of carbonyl and carboxyl groups. Figure 2c and 2d show the
characteristic bands, corresponding to PSS and Nafion.
In figure 2, we know that there are considerable changes in FT-IR spectra of GO after
treatment with hydrazine hydrate. The hydrazine hydrate treatment eliminated all of GO
bands, giving evidence for the almost removal of the oxygen-containing groups (figure 2b,
2c, 2d). As a result of this, the graphene was prepared by chemical reduction in aqueous
polymer solution, PSS or Nafion.
Graphene – Synthesis, Characterization, Properties and Applications40
4000 3500 3000 2500 2000 1500 1000 500
W avenumber (cm-1)
Fig. 2. FT-IR spectra in KBr of the samples GO (a), RGO (b), RGO-PSS (c), RGO-Nafion (d)
Figure 3 shows the UV/Vis spectra of polymer-coated RGO in water. RGO-PSS has two
absorption peaks in the UV/Vis spectrum. The absorption at 230 nm ascribed to the PSS
and that at 280 nm to reduced graphite oxide. It is known that the peak at 280 nm is the
characteristic peak of graphite in solution. The intensities of the signal of the polymers
(PSS and Nafion) are also small, indicating the polymer is strongly attached to the
graphene surface . In figure 3(b), Nafion-coated graphene show only the peak of the
RGO. Due to the higher absorbance of RGO, Nafion peak may be getting masked in the
spectrum, because there is not the absorption peak in UV/Vis spectrum of nafion. In
figure 3, RGO-PSS and RGO-Nafion have all the characteristic peak of RGO. This shows
that polymer-coated graphene have the stable state in the water solution. The chemical
composition of both PSS- and Nafion-coated graphene was monitored by X-Ray
photoelectron spectroscopy (XPS). Figure 4 shows XPS analysis of graphite oxide and
polymer-coated graphenes. The C 1s XPS spectrum of GO indicates a considerable degree
of oxidation with four major signatures corresponding to carbon atoms in different
functional groups. They are non-oxygenated ring C at 284.8 eV, C of C-O bonds at
286.1 eV, C of C=O at 287.3 eV, and that of carboxylate carbon (O-C=O) at 289.0 eV .
Oxygen functionalities of the graphite oxide were decreased during the reduction
progressed. C 1s XPS of RGO-PSS and RGO-Nafion also showed similar to spectra of GO.
However the intensities of oxygenated carbon peaks are considerably decreased, implying
reduction. In addition, there is an additional component at 285.8 eV corresponding to
C bound to nitrogen of hydrazones. The C 1s XPS spectrum of the Nafion-coated reduced
graphite oxide sample also contains a component peak at 292.7 eV corresponding to the
fluorine-bonded carbon atoms from Nafion.
Synthesis of Aqueous Dispersion of Graphenes via
Reduction of Graphite Oxide in the Solution of Conductive Polymer 41
Fig. 3. UV-Vis spectra of the polymer-coated graphene. PSS-RGO (a), Nafion-RGO (b).
200 250 300 350 400 450 500
200 300 400 500 600 700
W avwlwngth (nm )
Graphene – Synthesis, Characterization, Properties and Applications42
Fig. 4. XPS analysis of graphite oxide (a), PSS-coated graphene (b), Nafion-coated graphene (c).
2 8 0 2 8 5 2 9 0 2 9 5
B in d in g e n e rg y (e V )
280 285 290 295
B inding energy (eV )
2 8 0 2 8 5 2 9 0 2 9 5
B in d in g e n e rg y (e V )
Synthesis of Aqueous Dispersion of Graphenes via
Reduction of Graphite Oxide in the Solution of Conductive Polymer 43
The conductivities of PEDOT films as a function of the graphene content were shown in
figure 5. The thickness of the films range 0.1 µm to 0.3 µm. As the polymer-coated graphene
content in PEDOT/PSS solution increase from 0 to 1.2wt%, the conductivity of graphene-
doped PEDOT film increases. The PEDOT/PSS film with RGO-Nafion increased
significantly from 0.25 S/cm for pure PEDOT film and reached 12 S/cm, and the film with
RGO-PSS showed 3.2 S/cm when graphene was doped to 1.2ⅹ10-3wt% in PEOT solution.
The conductivity of PEDOT doped Nafion-coated graphene were increased approximately
60-fold than the origin PEDOT film. This indicates that the doped graphene strongly
influences the conductivity of PEDOT film. The film of PEDOT doped with RGO-Nafion
had also higher conductivities than films doped with RGO-PSS. It is known that Nafion has
ionic conductive property and PSS is the insulating material. As a result, it implies that the
graphene coated with ionic conductive material contributes to enhancement of conductivity
than that coated insulating material.
0.0 0.2 0.4 0.6 0.8 1.0 1.2 1.4
Concentration of graphite in solution (X10
Fig. 5. Conductivity of PEDOT films with varying doping content
In this study, we carried to the reduction of graphite oxide in the soluble Nafion, ionic
conductive polymer. Reduced graphite was not dispersed in water but polymer-coated
graphenes (RGO-PSS and RGO-Nafion) were dispersed readily in water, and readily forms
stable dispersed state. There are considerable changes in FT-IR spectra of GO after treatment
with hydrazine hydrate, implying successful reduction of graphite oxide in aqueous
solution of Nafion. UV/Vis spectrum of RGO-Nafion is similar to the characteristic peak of
RGO. It indicated that Nafion-coated graphene have the stable state in the water solution.
Graphene – Synthesis, Characterization, Properties and Applications44
The PEDOT film with Nafion-coated graphene increased significantly from 0.25 S/cm for
pure PEDOT film and reached 12 S/cm. The film of PEDOT doped Nafion-coated graphene
had also higher conductivities than films doped PSS-coated graphene.
Hong, W.; Xu Y.; Lu G.; Li C.& Shi G. (2008) Electrochemistry Comm., Vol.10, pp. 1555-1558,
Novoselov, K.S.; Geim, A.K.; Morozov, S.V.; Jiang, D.; Zheng, Y.; Dubonos, S.V; Grigorieva,
I.V. & Firsov A.A. (2004) Science, Vol.306 pp. 666, ISSN 0036-8075
Li, D.M. ; Muller, M.B. ; Gilje, S. ; Kanner, R.B. & Wallace, G.G. (2008) Nat. Nanotechnol. Vol.3
pp. 101-105, ISSN 1748-3387
Stankovich, S. ; Piner, R.D. ; Nfuyen, S.T. & Ruoff, R.S. (2006) Carbon, Vol.44 pp. 3342-3347,
Brodie, B.C. (1960) Ann. Chim. Phys., Vol.59 pp. 466-472
Hua, L. ; Kai, W. & Inoue, Y. (2007) J. Appl. Polym. Sci., Vol.106 pp. 1880-1884, ISSN 1097-
Becerril, H.A. ; Mao, J. ; Liu, Z. ; Stoltenberg, R.M. ; Bao, Z. & Chen, Y. (2008) ACS Nano,
Vol.2 pp. 463-470, ISSN 1936-0851
Stankovich, S. ; Piner, R.D. ; Chen, X. ; Wu, N. ; Nguyen, S.T. & Ruoff, R.S. (2006) J. Matter.
Chem., Vol.16 pp. 155-158, ISSN 0959-9428
Chen, G.; Weng, W.; Wu, D. & Wu, C. (2003) European Polymer Journal, Vol.39 pp. 2329-2335,
Hummers, W.S. & Offeman, R.E. (1958) J. Am. Chem. Soc., Vol.80 pp. 1339, ISSN 0002-7863
Stankovich, S. ; Dikin, D.A. ; Piner, R.D. ; Kohlhaas, K.A. ; Kleinhammes, A. ; Jia, Y. ; Wu, Y. ;
Nguyen, S.T. & Ruoff, R.S. (2007) Carbon, Vol.45 pp. 1558-156, ISSN 0008-6223
Supercritical Fluid Processing of
Graphene and Graphene Oxide
Dinesh Rangappa, Ji-Hoon Jang and Itaru Honma
Institute of Multidisciplinary Research for Advanced Materials,
Tohoku University, Katahira, Aoba-ku, Sendai,
Graphene which is single or few atomic layer carbon atoms in a hexagonal network is
emerging as a leader among the 2D nanoscale materials . Structurally, graphene is free of
defects, with all the carbon atoms linked together by strong and flexible bonds. This has made
graphene to have unusual electronic, optical, mechanical and thermal properties. The
outstanding properties of graphene reported so far includes Young’s modulus (~1100Gpa),
fracture strength (125 Gpa), high thermal conductivity (~ 5000 W m-1K-1), quantum Hall effect
at room temperature [2–4], an ambipolar electric field effect along with ballistic conduction of
charge carriers , tunable band gap and so on. Many efforts have been made on the
preparation of the graphene via a number of physical and chemical methods. Some of these
methods provides high quality graphene and has opened up new possible routes to address
the challenges in preparation and molecular engineering of high quality processable graphene
at low cost and large scale . In spite of this progress, the standard procedure to make the
high quality graphene is micromechanical cleavage method, which is suitable for only
fundamental studies . Alternatively, selective epitaxial growth of graphene on metal or
nonmetal substrates using chemical vapor deposition or by thermal decomposition of SiC was
developed . The graphene-type carbon materials have been produced by substrate free CVD
and radio-frequency plasma-enhanced CVD and so on . On the other hand, the chemical
routes are widely considered as a promising approach for large scale production . This
approach provides processable graphene, that can be easily cast into various structures or
integrate graphene with other materials to form nanocomposites [8, 9]. Currently, there are
two most popular chemical approaches to obtain graphene: dispersion and exfoliation of
graphite/graphene oxide/graphite intercalation compounds and its reduction after exfoliation
or direct exfoliation without chemical modification in suitable organic solvents or surfactants
. Unlike the direct exfoliation approach, the chemical modification method results in
considerable destruction of graphene electronic structure, thus compromising its unique
properties [10, 11]. In addition, these methods involve several steps and need 3-5 days to allow
the intercalants and organic solvents to fully insert into the graphitic layers .
In contrast to this oxidation and reduction method, some people have developed direct
graphite exfoliation method using suitable organic solvent. A high quality single layer
graphene sheets (GS) have been prepared by the chemical solution process in which
graphite was directly exfoliated in an organic solvent such as N-methylpyrrolidone (NMP)
Graphene – Synthesis, Characterization, Properties and Applications46
under mild sonication . In this work Coleman and co-workers have demonstrated that it
is possible to effectively exfoliate graphite to produce single and few-layer GSs without the
use of intercalants. The key to this success was the proper solvents for which the solvent–
graphene interfacial interaction energy matches that of graphene–graphene. This method
could produce a stable dispersion of graphene with the concentration of ~0.01mg/ml with a
monolayer yield of ~1 wt%. This monolayer yield could potentially be improved to ~7–12
wt% with further processing. This approach resulted in the high quality graphene without
any defects or oxides on the surface, which was completely different from that of the other
solution method such as, graphite oxidation and reduction approach. Later, same group has
developed a method to disperse and exfoliate graphite to give graphene suspended in
water-surfactant solutions . By Transmission electron microscopy, they had confirmed
that the dispersed phase was mainly consisting of small graphitic flakes, in which more than
40% of these flakes had <5 layers with ~3% of flakes consisting of monolayer. Atomic
resolution transmission electron microscopy shows the monolayer to be generally free of
defects. The dispersed graphitic flakes are stabilized against the aggregation by Coulomb
repulsion due to the adsorbed surfactant.
Few researchers have reported an environment-friendly method to produce graphene. For
example, Loh et al. presented a green approach for reduction of graphite oxide to graphene
using hydrothermal dehydration method . Zheng et al. has reported solvothermal route to
prepare graphene by direct exfoliation using oleylamine as a solvent as well as stabilizing
agent . Nuvoli et al has used a commercial ionic liquid 1-hexyl-3-methylimidazolium
hexafluorophosphate (HMIH), as a convenient solvent medium for graphite exfoliation in mild
and easy conditions without any chemical modification . This method resulted in few layer
graphene with a concentration as high as 5.33 mg/ml, which is the highest value reported so
far in any solvent. However, most of these methods take long reaction time and some time
they need size separation process in order to remove unexfoliated large graphite flakes.
On the other hand, the supercritical fluids (SCFs) have been widely studied as a new kind of
reaction media for nanomaterials synthesis owing to their unique properties such as; gas
like diffusivity, low viscosity and the density closer to that of liquid [18-20]. The SCFs have
much more empty space than ordinary liquids and are highly compressible. Consequently,
the density and hence “the solvent strength” of the fluid may be tuned from “gas-like” to
“liquid-like” values simply by varying pressure, temperature, or both. This tunability, along
with low interfacial tension, excellent wetting of surfaces, and high diffusion coefficients,
makes supercritical fluids potentially superior solvent for diffusion in between the layers
and its expansion. Taking advantage of these unique properties of SCFs, recently, we have
developed a novel SCF method for the exfoliation of graphite to obtain the high quality and
high yielding graphene sheets . This rapid and facile one-pot exfoliation method
resulted in highly conductive GS maintaining its original nature, although a high
temperature and pressure were used to create a suitable environment for SCF exfoliation.
Direct high-yield conversion of graphite crystals to GS was possible under SCF conditions
because of the high diffusivity and solvating power of SCFs, such as ethanol, N-methyl-
pyrrolidone (NMP), and DMF.
Currently, the focus has been shifted considering the graphene as ideal 2D materials to
understand the fundamental physics to its treatment as a large carbon macromolecule which
offers new promise . Years of research on carbon nanotube, fullerene, and graphite have
produced a myriad of chemical pathways for modifying sp2 carbon structures, which will
undoubtedly be adapted to functionalize both the basal plane of graphene and its reactive